Four-point flexural test. The four-point flexural test provides values for the modulus of elasticity in bending , flexural stress , flexural strain  and the flexural stress-strain response of the material. This test is very similar to the three-point bending flexural test. The major difference being that with the addition of a fourth bearing the portion of the beam between the two loading points is put under maximum stress, as opposed to only the material right under the central bearing in the case of three-point bending.

This difference is of prime importance when studying brittle materials, where the number and severity of flaws exposed to the maximum stress is directly related to the flexural strength and crack initiation. Compared to the three-point bending flexural test, there are no shear forces in the four-point bending flexural test in the area between the two loading pins. The four-point bending test is therefore particularly suitable for brittle materials that cannot withstand shear stresses very well.

It is one of the most widely used apparatus to characterize fatigue and flexural stiffness of asphalt mixtures.

Testing method 
The test method for conducting the test usually involves a specified test fixture on a universal testing machine.  Details of the test preparation, conditioning, and conduct affect the test results. The sample is placed on two supporting pins a set distance apart and two loading pins placed at an equal distance around the center. These two loadings are lowered from above at a constant rate until sample failure.

Calculation of the flexural stress 

  for four-point bending test where the loading span is 1/2 of the support span (rectangular cross section)

  for four-point bending test where the loading span is 1/3 of the support span (rectangular cross section)

  for three-point bending test (rectangular cross section)

in these formulas the following parameters are used:
   = Stress in outer fibers at midpoint, (MPa)
    = load at a given point on the load deflection curve, (N)
    = Support span, (mm)
    = Width of test beam, (mm)
    = Depth or thickness of tested beam, (mm)

Calculation of the Elastic modulus  
In the 4-point bending test, the specimen is placed on two supports and loaded in the middle by a test punch with two loading points. This results in a constant bending moment between the two supports. Consequently, a shear-free zone is created, where the specimen is subjected only to bending. This has the advantage that no additional shear force acts on the specimen, unlike in the 3-point bending test.

The bending modulus for a flat specimen is calculated as follows:

b: Specimen width in mm
a: Specimen thickness in mm
lA: Span length (distance between support point and the nearest loading point of the test punch) in mm
lB: Length of the reference beam (between the loading points, symmetrically placed relative to the loading points) in mm
DL: Distance between the reference beam and the main beam (centered between the loading points) in mm
E: Bending modulus in kN/mm²
lv: Span length in mm
XH: End of bending modulus determination in kN
XL: Start of bending modulus determination in kN
DL: Deflection in mm between XH and XL

Advantages and disadvantages 
Advantages of three-point and four-point bending tests over uniaxial tensile tests include:
 simpler sample geometries
 minimum sample machining is required
 simple test fixture
 possibility to use as-fabricated materials

Disadvantages include:
 more complex integral stress distributions through the sample

Application with different materials

Ceramics 
Ceramics are usually very brittle, and their flexural strength depends on both their inherent toughness and the size and severity of flaws. Exposing a large volume of material to the maximum stress will reduce the measured flexural strength because it increases the likelihood of having cracks reaching critical length at a given applied load. Values for the flexural strength measured with four-point bending will be significantly lower than with three-point bending., Compared with three-point bending test, this method is more suitable for strength evaluation of butt joint specimens. The advantage of four-point bending test is that a larger portion of the specimen between two inner loading pins is subjected to a constant bending moment, and therefore, positioning the joint region is more repeatable.

Composite materials

Plastics

Standards 

 ASTM C1161: Standard Test Method for Flexural Strength of Advanced Ceramics at Ambient Temperature

 ASTM D6272: Standard Test Method for Flexural Properties of Unreinforced and Reinforced Plastics and Electrical Insulating Materials by Four-Point Bending

 ASTM C393: Standard Test Method for Core Shear Properties of Sandwich Constructions by Beam Flexure
 ASTM D7249: Standard Test Method for Facing Properties of Sandwich Constructions by Long Beam Flexure
 ASTM D7250: Standard Practice for Determining Sandwich Beam Flexural and Shear Stiffness

See also 
Bending
Euler–Bernoulli beam equation
Flexural strength
Three-point flexural test
List of area moments of inertia
Second moment of area

References

External links

 ASTM C1161: Standard Test Method for Flexural Strength of Advanced Ceramics at Ambient Temperature

 ASTM D6272: Standard Test Method for Flexural Properties of Unreinforced and Reinforced Plastics and Electrical Insulating Materials by Four-Point Bending

 ASTM C393: Standard Test Method for Core Shear Properties of Sandwich Constructions by Beam Flexure
 ASTM D7249: Standard Test Method for Facing Properties of Sandwich Constructions by Long Beam Flexure
 ASTM D7250: Standard Practice for Determining Sandwich Beam Flexural and Shear Stiffness
 ASTM C78: Standard Test Method for Flexural Strength of Concrete (Using Simple Beam with Third-Point Loading)

Materials testing
Mechanics